LMucko/crystallography-open-database huggingface dataset:
Atomic ordering in binary A15-type phases
van Reuth, E.C.; Waterstrat, R.M.; Acta Crystallographica B (24,1968-38,1982) 24 (1968) 186–196; doi:

data_2107216
_publ_section_title
;
 Atomic ordering in binary A15-type phases
;
_journal_name_full               'Acta Crystallographica B (24,1968-38,1982)'
_journal_page_first              186
_journal_page_last               196
_journal_volume                  24
_journal_year                    1968
_chemical_formula_sum            'Mo6.4 Pt1.6'
_chemical_name_systematic        '(Mo4 Pt)1.6'
_space_group_IT_number           223
_symmetry_space_group_name_Hall  '-P 4n 2 3'
_symmetry_space_group_name_H-M   'P m -3 n'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   4.9878
_cell_length_b                   4.9878
_cell_length_c                   4.9878
_cell_volume                     124.087
_citation_journal_id_ASTM        ACBCAR
_cod_data_source_file            vanReuth_ACBCAR_1968_710.cif
_cod_data_source_block           Mo6.4Pt1.6
_cod_original_cell_volume        124.0872
_cod_database_code               2107216
Single uranium-site properties of the dilute heavy electron system Ux Th1-x Ru2 Si2 (x= 0.07)
Amitsuka, H.; Sakakibara, T.; Journal of the Physical Society of Japan 63 (1994) 736–747; doi:

data_1539564
_publ_section_title
;
 Single uranium-site properties of the dilute heavy electron system Ux
 Th1-x Ru2 Si2 (x= 0.07)
;
_journal_name_full               'Journal of the Physical Society of Japan'
_journal_page_first              736
_journal_page_last               747
_journal_volume                  63
_journal_year                    1994
_chemical_formula_sum            'Ru2 Si2 Th0.9 U0.1'
_chemical_name_systematic        'Ru2 (Th0.9 U0.1) Si2'
_space_group_IT_number           139
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   4.192
_cell_length_b                   4.192
_cell_length_c                   9.738
_cell_volume                     171.125
_citation_journal_id_ASTM        JUPSAU
_cod_data_source_file            Amitsuka_JUPSAU_1994_1119.cif
_cod_data_source_block           Ru2Si2Th0.9U0.1
_cod_original_cell_volume        171.1245
_cod_database_code               1539564
Etude de combinaisons entre divers sulfures de lanthanides (et d'yttrium): systemes L S-L2 S3, Cs S-L S, Ce S-L2 S3, Er2 S3-L2 S3, Er5 S7-L5 S7, Er3 S4-L3 S4
van Tien, V.; Khodadad, P.; Bulletin de la Societe Chimique de France (Vol=Year) 1969 (1969) 30–39; doi:

data_1539565
_publ_section_title
;
 Etude de combinaisons entre divers sulfures de lanthanides (et
 d'yttrium): systemes L S-L2 S3, Cs S-L S, Ce S-L2 S3, Er2 S3-L2 S3, Er5
 S7-L5 S7, Er3 S4-L3 S4
;
_journal_name_full
'Bulletin de la Societe Chimique de France (Vol=Year)'
_journal_page_first              30
_journal_page_last               39
_journal_volume                  1969
_journal_year                    1969
_chemical_formula_sum            'La3 S4'
_space_group_IT_number           220
_symmetry_space_group_name_Hall  'I -4bd 2c 3'
_symmetry_space_group_name_H-M   'I -4 3 d'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   8.73
_cell_length_b                   8.73
_cell_length_c                   8.73
_cell_volume                     665.339
_citation_journal_id_ASTM        BSCFAS
_cod_data_source_file            vanTien_BSCFAS_1969_439.cif
_cod_data_source_block           La3S4
_cod_original_cell_volume        665.3385
_cod_database_code               1539565
Stability range, structure and magnetic properties of Y Fe12-x Mox (0.5 <= x <= 2.0) alloys
Anagnostou, M.; Psycharis, V.; Devlin, E.; Kostikas, A.; Niarchos, D.; Journal of Magnetism and Magnetic Materials 131 (1994) 157–166; doi:

data_1539566
_publ_section_title
;
 Stability range, structure and magnetic properties of Y Fe12-x Mox (0.5
 <= x <= 2.0) alloys
;
_journal_name_full               'Journal of Magnetism and Magnetic Materials'
_journal_page_first              157
_journal_page_last               166
_journal_volume                  131
_journal_year                    1994
_chemical_formula_sum            'Fe22.5 Mo1.5 Y2'
_chemical_name_systematic        '(Fe45 Mo3 Y4)0.5'
_space_group_IT_number           139
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   8.5036
_cell_length_b                   8.5036
_cell_length_c                   4.7778
_cell_volume                     345.489
_citation_journal_id_ASTM        JMMMDC
_cod_data_source_file            Anagnostou_JMMMDC_1994_1056.cif
_cod_data_source_block           Fe22.5Mo1.5Y2
_cod_original_cell_volume        345.4885
_cod_database_code               1539566
Influence of radius ratio on the structure of intermetallic compounds of the AB3 type
van Vucht, J.H.N.; Journal of the Less-Common Metals 11 (1966) 308–322; doi:

data_1539567
_publ_section_title
;
 Influence of radius ratio on the structure of intermetallic compounds of
 the AB3 type
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              308
_journal_page_last               322
_journal_volume                  11
_journal_year                    1966
_chemical_formula_sum            'In3 Th'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   4.96
_cell_length_b                   4.96
_cell_length_c                   4.96
_cell_volume                     122.024
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            vanVucht_JCOMAH_1966_302.cif
_cod_data_source_block           In3Th1
_cod_original_cell_volume        122.0239
_cod_original_formula_sum        'In3 Th1'
_cod_database_code               1539567
Stability range, structure and magnetic properties of Y Fe12-x Mox (0.5 <= x <= 2.0) alloys
Anagnostou, M.; Devlin, E.; Kostikas, A.; Psycharis, V.; Niarchos, D.; Journal of Magnetism and Magnetic Materials 131 (1994) 157–166; doi:

data_1539568
_publ_section_title
;
 Stability range, structure and magnetic properties of Y Fe12-x Mox (0.5
 <= x <= 2.0) alloys
;
_journal_name_full               'Journal of Magnetism and Magnetic Materials'
_journal_page_first              157
_journal_page_last               166
_journal_volume                  131
_journal_year                    1994
_chemical_formula_sum            'Fe11 Mo Y'
_space_group_IT_number           139
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.5159
_cell_length_b                   8.5159
_cell_length_c                   4.7805
_cell_volume                     346.685
_citation_journal_id_ASTM        JMMMDC
_cod_data_source_file            Anagnostou_JMMMDC_1994_1057.cif
_cod_data_source_block           Fe11Mo1Y1
_cod_original_cell_volume        346.6845
_cod_original_formula_sum        'Fe11 Mo1 Y1'
_cod_database_code               1539568
Influence of radius ratio on the structure of intermetallic compounds of the AB3 type
van Vucht, J.H.N.; Journal of the Less-Common Metals 11 (1966) 308–322; doi:

data_1539569
_publ_section_title
;
 Influence of radius ratio on the structure of intermetallic compounds of
 the AB3 type
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              308
_journal_page_last               322
_journal_volume                  11
_journal_year                    1966
_chemical_formula_sum            'La Pb3'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   4.941
_cell_length_b                   4.941
_cell_length_c                   4.941
_cell_volume                     120.627
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            vanVucht_JCOMAH_1966_418.cif
_cod_data_source_block           La1Pb3
_cod_original_formula_sum        'La1 Pb3'
_cod_database_code               1539569
Stability range, structure and magnetic properties of Y Fe12-x Mox (0.5 <= x <= 2.0) alloys
Anagnostou, M.; Kostikas, A.; Psycharis, V.; Devlin, E.; Niarchos, D.; Journal of Magnetism and Magnetic Materials 131 (1994) 157–166; doi:

data_1539570
_publ_section_title
;
 Stability range, structure and magnetic properties of Y Fe12-x Mox (0.5
 <= x <= 2.0) alloys
;
_journal_name_full               'Journal of Magnetism and Magnetic Materials'
_journal_page_first              157
_journal_page_last               166
_journal_volume                  131
_journal_year                    1994
_chemical_formula_sum            'Fe10 Mo2 Y'
_space_group_IT_number           139
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.5516
_cell_length_b                   8.5516
_cell_length_c                   4.7985
_cell_volume                     350.914
_citation_journal_id_ASTM        JMMMDC
_cod_data_source_file            Anagnostou_JMMMDC_1994_1058.cif
_cod_data_source_block           Fe10Mo2Y1
_cod_original_cell_volume        350.9137
_cod_original_formula_sum        'Fe10 Mo2 Y1'
_cod_database_code               1539570
Note on the occurrence of intermetallic compounds in the lithium-palladi-um system
van Vucht, J.H.N.; Buschow, K.H.J.; Journal of the Less-Common Metals 48 (1976) 345–347; doi:

data_1539571
_publ_section_title
;
 Note on the occurrence of intermetallic compounds in the
 lithium-palladi-um system
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              345
_journal_page_last               347
_journal_volume                  48
_journal_year                    1976
_chemical_formula_sum            'Li Pd'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   2.977
_cell_length_b                   2.977
_cell_length_c                   2.977
_cell_volume                     26.384
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            vanVucht_JCOMAH_1976_498.cif
_cod_data_source_block           Li1Pd1
_cod_original_cell_volume        26.38375
_cod_original_formula_sum        'Li1 Pd1'
_cod_database_code               1539571
The structure of K2 Te O3 - an experimental and theoretical study
Andersen, L.; Langer, V.; Stroemberg, A.; Stroemberg, D.; Acta Crystallographica B (39,1983-) 45 (1989) 344–348; doi:

data_2107217
_publ_section_title
;
 The structure of K2 Te O3 - an experimental and theoretical study
;
_journal_name_full               'Acta Crystallographica B (39,1983-)'
_journal_page_first              344
_journal_page_last               348
_journal_volume                  45
_journal_year                    1989
_chemical_formula_sum            'K2 O3 Te'
_chemical_name_systematic        'K2 (Te O3)'
_space_group_IT_number           147
_symmetry_space_group_name_Hall  '-P 3'
_symmetry_space_group_name_H-M   'P -3'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   6.279
_cell_length_b                   6.279
_cell_length_c                   7.069
_cell_volume                     241.362
_citation_journal_id_ASTM        ASBSDK
_cod_data_source_file            Andersen_ASBSDK_1989_690.cif
_cod_data_source_block           K2O3Te1
_cod_original_cell_volume        241.3624
_cod_original_formula_sum        'K2 O3 Te1'
_cod_database_code               2107217
The crystal structure of K3 V S4
van den Berg, J.M.; de Vries, R.; Koninklijke Nederlandse Akademie van Wetenschappen, Series B: Physical Sciences: Proceedings 67 (1964) 178–180; doi:

data_1539572
_publ_section_title
;
 The crystal structure of K3 V S4
;
_journal_name_full
;
Koninklijke Nederlandse Akademie van Wetenschappen, Series B: Physical 
Sciences: Proceedings
;
_journal_page_first              178
_journal_page_last               180
_journal_volume                  67
_journal_year                    1964
_chemical_formula_sum            'K3 S4 V'
_chemical_name_systematic        'K3 V S4'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.143
_cell_length_b                   10.59
_cell_length_c                   9.107
_cell_volume                     881.780
_citation_journal_id_ASTM        KNWBAA
_cod_data_source_file            vandenBerg_KNWBAA_1964_380.cif
_cod_data_source_block           K3S4V1
_cod_original_cell_volume        881.7795
_cod_original_formula_sum        'K3 S4 V1'
_cod_database_code               1539572
Structural study of Mg-exchanged NaX and CaX zeolites in hydrated (25oC) and dehydrated (400oC) states
Anderson, A.A.; Shepelev, Yu.F.; Smolin, Yu.I.; Zeolites 10 (1990) 32–37; doi:

data_1539573
_publ_section_title
;
 Structural study of Mg-exchanged NaX and CaX zeolites in hydrated (25oC)
 and dehydrated (400oC) states
;
_journal_name_full               Zeolites
_journal_page_first              32
_journal_page_last               37
_journal_volume                  10
_journal_year                    1990
_chemical_formula_sum            'Al92 H212.48 Mg19.2 Na26.88 O490.24 Si100'
_chemical_name_systematic
'Mg19.2 Na26.88 (Al92 Si100 O384) (H2 O)106.24'
_space_group_IT_number           203
_symmetry_space_group_name_Hall  '-F 2uv 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   25.06
_cell_length_b                   25.06
_cell_length_c                   25.06
_cell_volume                     15737.770
_citation_journal_id_ASTM        ZEOLD3
_cod_data_source_file            Anderson_ZEOLD3_1990_1378.cif
_cod_data_source_block           H212.48Al92Mg19.2Na26.88O490.24Si100
_cod_original_cell_volume        15737.77
_cod_original_formula_sum        'H212.48 Al92 Mg19.2 Na26.88 O490.24 Si100'
_cod_database_code               1539573
Lattice constants and Brillouin zone overlap in dilute magnesium alloys
von Batchelder, F.W.; Raeuchle, R.F.; Physical Review (1,1893-132,1963/141,1966-188,1969) 105 (1957) 59–61; doi:

data_1539574
_publ_section_title
;
 Lattice constants and Brillouin zone overlap in dilute magnesium alloys
;
_journal_name_full
'Physical Review (1,1893-132,1963/141,1966-188,1969)'
_journal_page_first              59
_journal_page_last               61
_journal_volume                  105
_journal_year                    1957
_chemical_formula_sum            'In0.212 Mg1.788'
_chemical_name_systematic        '(In Mg9)0.2'
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   3.1962
_cell_length_b                   3.1962
_cell_length_c                   5.2146
_cell_volume                     46.134
_citation_journal_id_ASTM        PHRVAO
_cod_data_source_file            vonBatchelder_PHRVAO_1957_231.cif
_cod_data_source_block           In0.212Mg1.788
_cod_original_cell_volume        46.13383
_cod_database_code               1539574
Structural study of Mg-exchanged NaX and CaX zeolites in hydrated (25oC) and dehydrated (400oC) states
Anderson, A.A.; Shepelev, Yu.F.; Smolin, Yu.I.; Zeolites 10 (1990) 32–37; doi:

data_1539575
_publ_section_title
;
 Structural study of Mg-exchanged NaX and CaX zeolites in hydrated (25oC)
 and dehydrated (400oC) states
;
_journal_name_full               Zeolites
_journal_page_first              32
_journal_page_last               37
_journal_volume                  10
_journal_year                    1990
_chemical_formula_sum            'Al92 Mg25.28 Na31.34 O384 Si100'
_chemical_name_systematic        'Mg25.28 Na31.34 (Al92 Si100 O384)'
_space_group_IT_number           203
_symmetry_space_group_name_Hall  '-F 2uv 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   24.78
_cell_length_b                   24.78
_cell_length_c                   24.78
_cell_volume                     15216.119
_citation_journal_id_ASTM        ZEOLD3
_cod_data_source_file            Anderson_ZEOLD3_1990_1379.cif
_cod_data_source_block           Al92Mg25.28Na31.34O384Si100
_cod_original_cell_volume        15216.12
_cod_database_code               1539575
Die Strukturen von Thuringit, Bavalit und Chamosit und ihre Stellung in der Chloritgruppe
von Engelhardt, W.; Zeitschrift fuer Kristallographie, Kristallgeometrie, Kristallphysik, Kristallchemie (-144,1977) 104 (1942) 142–159; doi:

data_8104288
_publ_section_title
;
 Die Strukturen von Thuringit, Bavalit und Chamosit und ihre Stellung in
 der Chloritgruppe
;
_journal_name_full
;
Zeitschrift fuer Kristallographie, Kristallgeometrie, Kristallphysik, 
Kristallchemie (-144,1977)
;
_journal_page_first              142
_journal_page_last               159
_journal_volume                  104
_journal_year                    1942
_chemical_formula_sum            'Al4.4 Fe7.9 H16 Mg1.5 O36 Si6.2'
_chemical_name_systematic
'(Mg1.5 Fe7.9 Al2.6) (Si6.2 Al1.8 O20) (O H)16'
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   5.401
_cell_length_b                   9.359
_cell_length_c                   14.028
_cell_volume                     709.087
_citation_journal_id_ASTM        ZEKGAX
_cod_data_source_file            vonEngelhardt_ZEKGAX_1942_1173.cif
_cod_data_source_block           H16Al4.4Fe7.9Mg1.5O36Si6.2
_cod_original_cell_volume        709.0868
_cod_original_formula_sum        'H16 Al4.4 Fe7.9 Mg1.5 O36 Si6.2'
_cod_database_code               8104288
Structural study of Mg-exchanged NaX and CaX zeolites in hydrated (25oC) and dehydrated (400oC) states
Anderson, A.A.; Shepelev, Yu.F.; Smolin, Yu.I.; Zeolites 10 (1990) 32–37; doi:

data_1539576
_publ_section_title
;
 Structural study of Mg-exchanged NaX and CaX zeolites in hydrated (25oC)
 and dehydrated (400oC) states
;
_journal_name_full               Zeolites
_journal_page_first              32
_journal_page_last               37
_journal_volume                  10
_journal_year                    1990
_chemical_formula_sum            'Al92 Ca18.56 H218.88 Mg8.64 O493.44 Si100'
_chemical_name_systematic
'Ca18.56 Mg8.64 (Al92 Si100 O384) (H2 O)109.44'
_space_group_IT_number           203
_symmetry_space_group_name_Hall  '-F 2uv 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   25.06
_cell_length_b                   25.06
_cell_length_c                   25.06
_cell_volume                     15737.770
_citation_journal_id_ASTM        ZEOLD3
_cod_data_source_file            Anderson_ZEOLD3_1990_1380.cif
_cod_data_source_block           H218.88Al92Ca18.56Mg8.64O493.44Si100
_cod_original_cell_volume        15737.77
_cod_original_formula_sum        'H218.88 Al92 Ca18.56 Mg8.64 O493.44 Si100'
_cod_database_code               1539576
Zur Kenntnis der Nitride der Cererden
von Essen, U.; Klemm, W.; Zeitschrift fuer Anorganische und Allgemeine Chemie 317 (1962) 25–34; doi:

data_1539577
_publ_section_title
;
 Zur Kenntnis der Nitride der Cererden
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              25
_journal_page_last               34
_journal_volume                  317
_journal_year                    1962
_chemical_formula_sum            'N Pr'
_chemical_name_systematic        'Pr N'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.302
_cell_length_b                   5.302
_cell_length_c                   5.302
_cell_volume                     149.046
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            vonEssen_ZAACAB_1962_766.cif
_cod_data_source_block           N1Pr1
_cod_original_cell_volume        149.0456
_cod_original_formula_sum        'N1 Pr1'
_cod_database_code               1539577
Structural study of Mg-exchanged NaX and CaX zeolites in hydrated (25oC) and dehydrated (400oC) states
Anderson, A.A.; Smolin, Yu.I.; Shepelev, Yu.F.; Zeolites 10 (1990) 32–37; doi:

data_1539578
_publ_section_title
;
 Structural study of Mg-exchanged NaX and CaX zeolites in hydrated (25oC)
 and dehydrated (400oC) states
;
_journal_name_full               Zeolites
_journal_page_first              32
_journal_page_last               37
_journal_volume                  10
_journal_year                    1990
_chemical_formula_sum            'Al92 Ca23.2 Mg22.4 O384 Si100'
_chemical_name_systematic        'Ca23.20 Mg22.4 (Al92 Si100 O384)'
_space_group_IT_number           203
_symmetry_space_group_name_Hall  '-F 2uv 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   24.92999
_cell_length_b                   24.92999
_cell_length_c                   24.92999
_cell_volume                     15494.099
_citation_journal_id_ASTM        ZEOLD3
_cod_data_source_file            Anderson_ZEOLD3_1990_1381.cif
_cod_data_source_block           Al92Ca23.2Mg22.4O384Si100
_cod_original_cell_volume        15494.1
_cod_database_code               1539578